Advances in Materials Science and Engineering
Volume 2018 (2018), Article ID 6842694, 6 pages
https://doi.org/10.1155/2018/6842694

Research Article

Influence of Temperature on the Performance of LiNi1/3Co1/3Mn1/3O₂ Prepared by High-Temperature Ball-Milling Method

Ming Tian,1,2 Xuetian Li,¹ Zhongbao Shao,² and Fengman Shen¹

¹School of Materials and Metallurgy, Northeastern University, Shenyang 110819, China
²College of Science, Northeastern University, Shenyang 110819, China

Correspondence should be addressed to Zhongbao Shao; shaozhongbao@mail.neu.edu.cn

Received 28 March 2017; Revised 10 July 2017; Accepted 25 October 2017; Published 15 January 2018

Academic Editor: Peter Majewski

Copyright © 2018 Ming Tian et al. This is an open access article distributed under the Creative Commons Attribution License, which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.

Abstract.

Aiming at the preparation of high electrochemical performance LiNi1/3Co1/3Mn1/3O₂ cathode material for lithium-ion battery, LiNi1/3Co1/3Mn1/3O₂ was prepared with lithium carbonate, nickel (II) oxide, cobalt (II, III) oxide, and manganese dioxide as raw materials by high-temperature ball-milling method. Influence of ball-milling temperature was investigated in this work. It was shown that the fine LiNi1/3Co1/3Mn1/3O₂ powder with high electrochemical performance can be produced by the high-temperature ball-milling process, and the optimal ball-milling temperature obtained in the current study was 750°C. Its initial discharge capacity was 146.0 mAhg⁻¹ at the rate of 0.1 C, and over 50 cycles its capacity retention rate was 90.2%.

1. Introduction

In the recent years, lithium-ion batteries have been widely used in small electronic devices because of their advantages in energy density and cycle life [1]. LiCoO₂ is generally employed as a cathode material, but co-bearing materials are expensive and could cause pollution issues. LiNiO₂ structure becomes unstable during the cell charging process as the material was delithiated. The instability of LiNiO₂ in lithiumion cells reduces the cycle life of the cell and leads to safety concerns [2]. Manganese cathode materials draw a lot of attention due to the advantages of low cost, abundant resources, and extensive distribution. LiMnO₂ is a kind of thermodynamic instable materials with high capacity. However, the layered structure is transformed into the spinel structure in the process of charge-discharge, leading to fast specific capacity attenuation and unstable electrochemical properties [3]. LiMn₂O₄ is prone to crystal transformation, solvation of manganese ion, and Jahn-Teller effect, leading to capacity fade in lithium batteries [4]. LiFeO₄ is regarded to be the zero pollution anode material, which has the advantage of cheap price and high security, but its application is limited due to the low conductivity and tap density [5, 6].

The layered ternary material which was first reported by Ohzuku and Makimura [7] cumulates the merits of LiCoO₂, LiNiO₂, and LiMnO₂. It is considered as one of the promising anode materials on account of high discharge specific capacity, static cycle life, low cost, and good safety performance [8].

Current methods for the large-scale preparation of high-performance cathode materials of three elements mainly include coprecipitation method [9–11] and solid-phase method [12–14]. The material synthesized by the solid-phase method has low impurity and capacity, while coprecipitation method could solve this problem. Some approaches such as sol-gel method, [15–17], microemulsion method [18], microwave method [19], spray pyrolysis [20], and combustion method [21] were studied in lab scale to prepare high-performance materials, but all these approaches are usually of high costs, have complicated processes, and are not environment-friendly.

High-temperature ball-milling method was modified from a traditional planetary mill by equipping controllable heating and automatic temperature-controlled elements; so, milling and sintering treatments could be simultaneously conducted in one reactor shortening the synthetic time [22–24]. In this work, LiNi1/3Co1/3Mn1/3O₂ powder was prepared by high-temperature ball-milling method with Li₂CO₃, NiO, Co₃O₄, and MnO₂ as raw materials, and the influence of milling temperature (700, 750, 800, and 850°C) on the product was investigated.

2. Experimental

A mass of 39.365 g lithium carbonate (Li₂CO₃, AR, 99.9%), 25.885 g nickel (II) oxide (NiO, CP, 99.5%), 27.677 g cobalt (II, III) oxide (Co₃O₄, AR, 99.9%), and 29.977 g manganese dioxide (MnO₂, AR, 99.9%) were dispersed in 250 mL boiling deionized water, which was agitated for 2 h at room temperature for intensive mixing. The precursor for LiNi1/3Co1/3Mn1/3O₂ was obtained after drying the product slurry at 120°C for 12 h. The HTBM was conducted in the novel mill, as illustrated in Figure 1(a). The precursor was poured into a jar with some milling balls at a ball-to-powder mass ratio of 15 : 1 followed by sealing of the mill [24]. The samples were heated to the set temperatures (700, 750, 800, and 850°C) and held at these temperatures for 12 h. A flow sheet of the process route is given in Figure 2.

Figure 1: Illustration of the high-temperature ball mill. (1) Support base, (2) temperature controller, (3) ball-milling canister, (4) grinding ball, (5) furnace body, (6) speed regulator, and (7) electrical motor.

Figure 2: Flow sheet of the process route.

The structure of LiNi1/3Co1/3Mn1/3O₂ was determined by X-ray diffraction (XRD) (Rigaku D/max-RB) with Cu-Kα radiation. The analysis was performed between 10° and 70° at a scan rate of 0.02°/min. The morphology and microstructure of the sample were characterized using scanning electron microscopy (SEM, HITACHI S-3000H) analysis.

The electrochemical performances of the samples were investigated using a two-electrode coin cell (CR2032). To prepare the working electrodes, 80% of LiNi1/3Co1/3Mn1/3O₂ powder, 10% of acetylene black, and 10% of polyvinylidene fluoride (PVDF) were dissolved in N-methyl pyrrolidone (NMP), and the electrode slurry was coated on an Al foil (the average weight of the active material in per piece of electrode was 6.7 mg) and then heated at 120°C under vacuum for 12 h. 1 M LiPF₆ in a mixture of ethylene carbonate (EC) and dimethyl carbonate (DMC) (1 : 1 in volume) was used as liquid electrolyte. Button batteries were assembled in argon-filled glove box with lithium metal as a counterelectrode and polypropylene (Celgard 2400) as a separator. Cycle charge-discharge tests at different rates were conducted using a NEWARE battery-testing system (Neware Co., Ltd., China) from 2.5 to 4.3 V at the room temperature (the current of 1 C equals to 200 mAhg⁻¹).

3. Results and Discussion

The XRD patterns of the resulting LiNi1/3Co1/3Mn1/3O₂ samples synthesized at different temperatures of 700, 750, 800, and 850°C for 12 h are shown in Figure 3. The diffraction peak intensity of LiNi1/3Co1/3Mn1/3O₂ was enhanced with the rise of ball-milling temperature, demonstrating that temperature has a great influence on the crystallinity of LiNi1/3Co1/3Mn1/3O₂. When the temperature was 700°C, some LiMn₂O₄ was generated, which is regarded as an impurity, showing that the reaction did not go completely. Diffraction peaks show a single phase of LiNi1/3Co1/3Mn1/3O₂ in an α-layered structure without any impurity phase when the temperature range is 750∼850°C.

Figure 3: XRD patterns of products prepared at various temperatures.

LiNi1/3Co1/3Mn1/3O₂ powder prepared at 700°C had unit cell parameters (Table 1) of a = 2.8642 Å and c = 14.18953 Å. LiNi1/3Co1/3Mn1/3O₂ powder prepared at 750°C had unit cell parameters of a = 2.8653 Å and c = 14.2384 Å. LiNi1/3Co1/3Mn1/3O₂ powder prepared at 800°C had unit cell parameters (Table 1) of a = 2.8661 Å and c = 14.2363 Å. LiNi1/3Co1/3Mn1/3O₂ powder prepared at 850°C had unit cell parameters (Table 1) of a = 2.8667 Å and c = 14.2295 Å. The ratio of c/a is usually used as a measurement of hexagonality for layered materials. When the ratio is greater than 4.9, it is assumed that the material possesses layered characteristics [25]. Table 1 shows that c/a of all the samples are greater than 4.9; it means all the samples possess layered characteristics.

Table 1: Lattice parameter of LiNi1/3Co1/3Mn1/3O₂ powders prepared at various temperatures.

N
a-axis (Å)
c-axis (Å)
c/a ratio

700°C
2.8642
14.1895
4.954

750°C
2.8653
14.2384
4.969

800°C
2.8661
14.2363
4.967

850°C
2.8667
14.2295
4.964

SEM images of the high-temperature ball-milling products prepared at different temperatures for 12 h are shown in Figure 4. It can be clearly found that some large particles were formed with the increase of temperature. When the temperature was 700°C, the product particles were small but in a severe agglomeration. When the temperature rose to 750°C, smaller spherical particles around 2–4 μm in length are obtained and the agglomeration was reduced. The grain sizes of the particles notably increased, and the agglomeration became more serious when the ball-milling process was conducted at 800 and 850°C.

(a)

(b)

(c)

(d)

Figure 4: SEM images of products prepared at various temperatures of (a) 700°C, (b) 750°C, (c) 800°C, and (d) 850°C.

The electrode characteristics of LiNi1/3Co1/3Mn1/3O₂ powder prepared at various ball-milling temperatures were examined by galvanostatic charge-discharge tests. The cell was cycled between 2.5 and 4.3 V using 0.1 C rate at room temperature. Figure 5(a) shows the initial charge-discharge curves of the four samples. Experimental results indicated that initial discharge capacities are 133.7, 161.8, 155.0, and 126.1 mAhg⁻¹, respectively, and the sample synthesized at 750°C has the highest capacity. The reason of this phenomenon include the following several aspects: some impurity of LiMn₂O₄ was generated when ball-milling process was carried out at 700°C, and when ball-milling temperatures were rose to 800 and 850°C, the grain sizes of the powder increased and the crystal agglomeration became serious. Therefore, the optimal ball-milling temperature for preparing LiNi1/3Co1/3Mn1/3O₂ powder obtained in the current study was 750°C.

(a)

(b)

(c)

Figure 5: (a) Charge-discharge curves of LiNi1/3Co1/3Mn1/3O₂ powders prepared at various temperatures: (A) 700°C, (B) 750°C, (C) 800°C, and (D) 850°C at 0.1 C rate, (b) discharge curves at various currents, and (c) the dependence of specific capacity on current density.

The rate performance at different currents of the LiNi1/3Co1/3Mn1/3O₂ powders prepared at 750°C is shown in Figure 5(b). Accordingly, the dependence of specific capacity on current density is given in Figure 5(c). The initial discharge capacities of the sample were 161.8, 152.7, 140.1, 129.2, and 116.4 mAhg⁻¹, at rates of 0.1, 0.2, 0.5, 1.0, and 2.0 C, respectively. When currents increased, the discharge capacities of the sample were slightly reduced. The initial discharge capacity was 116.4 mAhg⁻¹ at the rate of 2.0 C, demonstrating that the LiNi1/3Co1/3Mn1/3O₂ powder synthesized at 750 °C had an excellent rate performance. The cyclic performance at the current of 0.1 C of the LiNi1/3Co1/3Mn1/3O₂ powder prepared at 750°C is shown in Figure 6. After 50 cycles, the capacity of LiNi1/3Co1/3Mn1/3O₂ powder was 146.0 mAhg⁻¹; the capacity retention rate achieved 90.2% showing an excellent rate cyclic performance.

Figure 6: The cyclic performance at a current of 0.1 C of LiNi1/3Co1/3Mn1/3O₂ powder prepared at 750°C.

It is reported that LiNi1/3Co1/3Mn1/3O₂ powder had been synthesized by many methods. LiNi1/3Co1/3Mn1/3O₂ powder was prepared at 900°C for 12 h by coprecipitation method [26]; LiNi1/3Co1/3Mn1/3O₂ powder was obtained at 500°C for 6 h and then at 900°C for 12 h by original wet-chemical route [27]; LiNi1/3Co1/3Mn1/3O₂ powder was synthesized at 800°C for 20 h via microwave-hydrothermal method [28]. In this work, LiNi1/3Co1/3Mn1/3O₂ powder with performance uniformity was synthesized at a ball-milling temperature of 750°C for 12 h. Its initial discharge specific capacity was 161.8 mAh/g at the rate of 0.1 C from 2.5 V to 4.3 V. It means that LiNi1/3Co1/3Mn1/3O₂ powder synthesized at 750°C for 12 h by high-temperature ball-milling method had an excellent electrochemical performance.

4. Conclusions

In this work, LiNi1/3Co1/3Mn1/3O₂ powder was prepared via high-temperature ball-milling method, and the effect of temperature on the LiNi1/3Co1/3Mn1/3O₂ powder was investigated. Results showed that the optimal ball-milling temperature for preparing LiNi1/3Co1/3Mn1/3O₂ powder obtained in the current study is 750°C. The products have an excellent electrochemical performance.

Compared to other methods, LiNi1/3Co1/3Mn1/3O₂ powder prepared by high-temperature ball-milling method needs lower temperature. Based on the findings of this study, it is suggested that preparation of LiNi1/3Co1/3Mn1/3O₂ powder by high-temperature ball milling is simple for equipment, suitable for mass production, and easy for realization of industrialization.

Conflicts of Interest

The authors declare that there are no conflicts of interest regarding the publication of this paper.

References

T. Ohzuku and R. J. Brodd, “An overview of positive-electrode materials for advanced lithium-ion batteries,” Journal of Power Sources, vol. 174, no. 2, pp. 449–456, 2007.

W. Li and J. C. Currie, “Influence of morphology on the stability of LiNiO₂,” Journal of Power Sources, vol. 81-82, pp. 44–48, 1999.

A. R. Armstrong and P. G. Bruce, “Synthesis of layered LiMnO₂ as an electrode for rechargeable lithium batteries,” Nature, vol. 381, no. 6582, pp. 499-500, 1996.

S. T. Myung, K. Izumi, S. Komaba, Y. K. Sun, H. Yashiro, and N. Kumagai, “Role of alumina coating on Li-Ni-Co-Mn-O particles as positive electrode material for lithium-ion batteries,” Chemistry of Materials, vol. 17, no. 14, pp. 3695–3704, 2005.

P. P. Prosini, M. Lisi, S. Scaccia, M. Carewska, F. Cardellini, and M. Pasquali, “Synthesis and characterization of amorphous hydrated LiFePO₄ and its electrode performance in lithium batteries,” Journal of Electrochemical Society, vol. 149, no. 3, pp. A297–A301, 2002.

J. M. Tarascon and M. Armand, “Issues and challenges facing rechargeable lithium batteries,” Nature, vol. 414, no. 6861, pp. 359–367, 2001.

T. Ohzuku and Y. Makimura, “Layered lithium insertion material of LiCo1/3Ni1/3-Mn1/3O₂ for lithium-ion batteries,” Chemistry Letters, vol. 30, no. 7, pp. 642-643, 2001.

H. Yoshizawa and T. Ohzuku, “An application of lithium cobalt nickel manganese oxide to high-power and high-energy density lithium-ion batteries,” Journal of Power Sources, vol. 174, no. 2, pp. 813–817, 2007.

Y. Chen, G. F. Xu, J. L. Li, Y. K. Zhang, Z. Chen, and F. Y. Kang, “High capacity 0.5Li₂MnO₃·0.5LiNi0.33Co0.33Mn0.33O₂ cathode material via a fast co-precipitation method,” Electrochimica Acta, vol. 87, pp. 686–692, 2013.

R. R. Zhao, Z. J. Chen, Y. Zhang, P. Du, and H. Y. Chen, “Ultrasonic/microwave-assisted co-precipitation method in the synthesis of Li1.1Mn0.433Ni0.233Co0.233O₂ cathode material for lithium-ion batteries,” Materials Letters, vol. 136, pp. 160–163, 2014.

L. W. Liang, K. Du, W. Lu, Z. D. Peng, Y. B. Cao, and G. R. Hu, “Synthesis and characterization of concentration-gradient LiNi0.6Co0.2Mn0.2O₂ cathode material for lithium ion batteries,” Journal of Alloys & Compounds, vol. 613, no. 2, pp. 296–305, 2014.

E. Y. Bang, D. R. Mumm, H. R. Park, and M. Y. Song, “Lithium nickel cobalt oxides synthesized from Li₂CO₃, NiO and Co₃O₄ by the solid-state reaction method,” Ceramics International, vol. 38, no. 5, pp. 3635–3641, 2012.

E. Y. Bang, D. R. Mumm, H. R. Park, and M. Y. Song, “Comparison of lithium nickel cobalt oxides synthesized from NiO, Co₃O₄, and LiOH·H₂O or Li₂CO₃ by solid-state reaction method,” Ceramics International, vol. 38, no. 7, pp. 5699–5705, 2012.

M. Y. Song, H. Rim, and H. R. Park, “Electrochemical characteristics of cobalt-substituted lithium nickel oxides synthesized from lithium hydro-oxide and nickel and cobalt oxides,” Ceramics International, vol. 38, no. 8, pp. 6591–6597, 2012.

Y. Zhao, G. Sun, and R. Wu, “Synthesis of nanosized Fe-Mn based Li-rich cathode materials for lithium-ion battery via a simple method,” Electrochimica Acta, vol. 96, no. 5, pp. 291–297, 2013.

T. L. Zhao, S. Chen, L. Li et al., “Synthesis, characterization, and electrochemistry of cathode material Li[Li0.2Co0.13Ni0.13Mn0.54]O₂ using organic chelating agents for lithium-ion batteries,” Journal of Power Sources, vol. 228, no. 11, pp. 206–213, 2013.

S. J. Shi, J. P. Tu, Y. Y. Tang, Y. Q. Zhang, X. L. Wang, and C. D. Gu, “Preparation and characterization of macroporous Li1.2Mn0.54Ni0.13Co0.13O₂ cathode material for lithium-ion batteries via aerogel template,” Journal of Power Sources, vol. 240, no. 1, pp. 140–148, 2013.

C. H. Lu and Y. K. Lin, “Microemulsion preparation and electrochemical characteristics of LiNi1/3Co1/3Mn1/3O₂ powders,” Journal of Power Sources, vol. 189, no. 1, pp. 40–44, 2009.

Q. W. Peng, Z. Y. Tang, L. Q. Zhang, and X. J. Liu, “Synthesize of layered Li(1.2+x)[Ni(0.25)Mn(0.75)](0.8-x)O₂(0≤x≤4/5) materials via microwave heating method and their electrochemical properties,” Journal of South China Normal University, vol. 44, pp. 2147–2151, 2009.

T. Li, X. H. Li, Z. X. Wang, and H. J. Guo, “A short process for the efficient utilization of transition-metal chlorides in lithium-ion batteries: a case of Ni0.8Co0.1Mn0.1O1.1 and LiNi0.8Co0.1Mn0.1O₂,” Journal of Power Sources, vol. 175, pp. 564–569, 2008.

M. Y. Song, I. H. Kwon, H. R. Park, and D. R. Mumm, “Electrochemical properties of lithium nickel oxide synthesized by the combustion method in an O₂ stream,” Ceramics International, vol. 38, no. 3, pp. 2443–2448, 2012.

Z. B. Shao, Q. W. Hao, and Z. C. Shao, High energy ball mill [P]

Q. Zhao, Z. B. Shao, C. J. Liu et al., “Preparation of Cu-Cr alloy powder by mechanical alloying,” Journal of Alloys & Compounds, vol. 607, no. 10, pp. 118–124, 2014.

L. Y. Jia, Z. B. Shao, Q. Lü, Y. W. Tian, and J. F. Han, “Preparation of red-emitting phosphor (Y, Gd) BO₃: EU³⁺ by high temperature ball milling,” Ceramics International, vol. 40, no. 1, pp. 739–743, 2014.

C. S. Kang and J. T. Son, “Synthesis and electrochemical properties of LiCo1/3Ni1/3Mn1/3O₂ cathode materials by electrospinning process,” Journal of Electroceramics, vol. 29, no. 4, pp. 235–239, 2012.

E. Shinova, R. Stoyanova, E. Zhecheva, G. F. Ortiz, P. Lavela, and J. L. Tirado, “Cationic distribution and electrochemical performance of LiCo1/3Ni1/3Mn1/3O₂ electrodes for lithium-ion batteries,” Solid State Ionics, vol. 179, no. 38, pp. 2198–2208, 2008.

Q. Su, Y. J Li, L. Li et al., “Synthesis and electrochemical properties of LiCo1/3Ni1/3Mn1/3O₂ via an original wet-chemical route for high voltage Li-ion batteries,” Materials Letters, vol. 198, pp. 180–183, 2017.

H. B. Ren, Y. R. Wang, D. C. Li, L. H. Ren, Z. Peng, and Y. Zhou, “Synthesis of LiCo1/3Ni1/3Mn1/3O₂ as a cathode material for lithium battery by the rheological phase method,” Journal of Power Sources, vol. 178, pp. 439–444, 2008.